Molybdenum-Based Catalytic Materials for Li – S Batteries:
Strategies, Mechanisms, and Prospects
Yuping Liu,* Zhihua Lin, Frederik Bettels, Zhenhu Li, Jingjing Xu, Yulin Zhang, Xu Li, Fei Ding, Shuangyi Liu,* and Lin Zhang*
The international market for energy storage systems (ESSs) has experienced rapid growth over the past few decades, however,
the state-of-the-art EESs cannot keep up with the demand for grid-connected stor- age systems.Thus, batteries with higher energy/power densities and lower produc- tion costs are urgently needed. Among var- ious battery candidates, Li–S battery is considered one of the most attractive choices, because of their high theoretical energy density (2600 Wh kg1, more than ﬁve times of the traditional lithium-ion (Li-ion) batteries). Furthermore, the sulfur cathode has the advantages of nat- ural abundance, environmental friendli- ness, and low cost. Nevertheless, there are still several challenges to be resolved, including, 1) the intrinsic poor electrical conductivities of sulfur and Li2S (51030 S cm1 and 1030 S cm1, respectively) hinder the electron transfer and slow down the reaction kinetics;
2) the large volumetric changes during the lithiation/delithiation of S/Li2S; 3) the shuttle effect of the soluble lithium polysulﬁde intermediates (LiPSs) leads to self-discharging and fast capacity decay; 4) the unstable solid elec- trolyte interfase (SEI) of Li anode during the cycling.[2b,3]
Tremendous efforts have been devoted to addressing these challenges over the past few decades. Many works focused on developing the conductive framework and the sulfur adsorbent.
A variety of carbon-based hosts with porous structures have been widely investigated to facilitate the electron transfer and physical conﬁnement of the soluble LiPSs. However, these strategies demonstrated only limited effects on suppressing the shuttle effect, due to the weak van der Waals interactions between the nonpolar carbon and the polar LiPSs.[3a,4] In this regard, the modiﬁcation of carbon-based host by using heteroatoms (e.g., N, O, P-doping) and polar adsorbents (e.g., metal oxides and metal sulﬁdes) were proposed. Although these approaches can efﬁciently suppress the shuttle effect, they do not yet meet the stringent demand for commercial applications.
Moreover, for a number of applications, the batteries need to achieve not only high energy density but also high-power density.
This is especially the case in contemporary electric vehicles (e.g., during acceleration and uphill driving) and in grid/home energy storage. Therefore, high sulfur mass loadings, low electrolyte/
sulfur (E/S) ratio, and large current density are also required for Li–S batteries. However, these working parameters exacerbate the intrinsic Li–S problems, for instance, the sluggish redox kinetics and shuttle effect will result in low sulfur Y. Liu, Z. Li, J. Xu, Y. Zhang, X. Li, S. Liu
Research Center for Electrochemical Energy Storage Technologies Chongqing Institute of Green and Intelligent Technology Chinese Academy of Sciences
Chongqing 400714, P. R. China
E-mail: email@example.com; firstname.lastname@example.org Y. Liu, Z. Lin, F. Bettels, F. Ding, L. Zhang
Institute of Solid State Physics Leibniz University Hannover 30167 Hannover, Germany
E-mail: email@example.com Y. Liu, Z. Lin, F. Bettels, F. Ding, L. Zhang
Laboratory of Nano and Quantum Engineering (LNQE) Leibniz University Hannover
Hannover 30167, Germany
The ORCID identiﬁcation number(s) for the author(s) of this article can be found under https://doi.org/10.1002/aesr.202200145.
© 2022 The Authors. Advanced Energy and Sustainability Research pub- lished by Wiley-VCH GmbH. This is an open access article under the terms of the Creative Commons Attribution License, which permits use, distribution and reproduction in any medium, provided the original work is properly cited.
Lithium–sulfur (Li–S) batteries are regarded as promising candidates for high-energy storage devices because of their high theoretical energy density (2600 Wh kg1). However, their practical applications are still hindered by a multitude of key challenges, especially the shuttle effect of soluble lithium poly- sulﬁdes (LiPSs) and the sluggish sulfur redox kinetics. To address these challenges, varieties of catalytic materials have been exploited to prevent the shuttle effect and accelerate the LiPSs conversion. Recently, molybdenum-based (Mo-based) catalytic materials are widely used as sulfur host materials, modiﬁed separators, and interlayers for Li–S batteries. They include the Mo sulﬁdes, diselenides, carbides, nitrides, oxides, phosphides, borides, and metal/single atoms/clusters. Here, recent advances in these Mo-based catalytic materials are comprehensively summarized, and the current challenges and prospects for designing highly efﬁ- cient Mo-based catalytic materials are highlighted, with the aim to provide a fundamental understanding of the sulfur reaction mechanism, and to guide the rational design of cathode catalysts for high-energy and long-life Li–S batteries.
utilization and poor Columbic efﬁciency (CE), especially during the oxidation/reduction processes between the liquid (LiPSs)/
solid (Li2S2/Li2S) phases. The high activation barrier of the Li2S reduction process accelerates the deposition of Li2S on the Li metal surface and hence causes the dramatical capacity decay within a limited cycling number.
In light of this, many research strategies shift from blocking the dissolution of LiPSs to accelerating the redox kinetics between the LiPSs and Li2S2/Li2S. These“electrocatalyst”mate- rials can decrease the activation energy of redox LiPSs and accel- erate the ions/electron transport.The shuttle effect is therefore greatly suppressed and the electrochemical performances are signiﬁcantly improved. This strategy has been applied to a num- ber of Li–S systems, including metal oxides,metal sulﬁdes,
metal nitrides, metal carbides, heterostructures, and single atoms. Interestingly, many of these electrocatalysts are molybdenum-based (Mo-based), including Mo sulﬁdes, dis- elenides, carbides, nitrides, oxides, phosphides, borides, and metal/single atoms/clusters. Although there have been excellent overall reviews on the electrocatalysts in Li–S batteries,[3e,15] a dedicated summary on the highly efﬁcient Mo-based catalysts in Li–S batteries does not yet exist. Therefore, this review aims to present a comprehensive and insightful overview of Mo-based catalysts. The current challenges and prospects in thisﬁeld are highlighted, providing a fundamental understanding of the sul- fur reaction mechanism and guiding the rational design of cath- ode catalysts for high-energy and long-life Li–S batteries.
2. Catalytic Materials for the Conversion of LiPSs
The utilization of sulfur as electrode material wasﬁrst presented by Herbet and Ulam in 1962.During the discharge, octasulfur proceeds through multiple steps
S8þ2e–! S82– (1)
Theﬁrst three steps correspond to the transformation from solid S8 to the liquid high-order lithium polysulﬁdes (LiPSs) (Li2Sx, 4≤x≤8) in the voltage proﬁle (2.3 V), and the LiPSs spe- cies produced in these steps are soluble in the electrolyte (Figure 1a). Although these three steps have relatively moderate reaction kinetics, large quantities of LiPSs in the electrolyte cause an increased electrolyte concentration, and further lead to a raised internal resistance and polarization of the Li–S batteries.
In addition, the dissolved LiPSs in the electrolyte will corrode the Li metal and form the insoluble Li2S2/Li2S on the Li surface. An enhanced reaction kinetics can effectively shorten the detention time of the soluble LiPSs in the cathode, thereby suppressing the dissolution of LiPSs and decreasing the loss of active materials (Figure 1b).[7,18]
The last two steps are related to the reduction of high-order LiPSs to solid Li2S2/Li2S. These conversions are much more difﬁcult due to the crystallization of ionically/electrically insulating Li2S2.The sluggish reaction kinetics in these steps leads to low sulfur utiliza- tion and limited discharge capacity (since these steps contribute about 75% speciﬁc capacity), thus the reversible speciﬁc capacity is strongly related to the reaction kinetics. Upon charging, the ioni- cally/electrically insulating Li2S2/Li2S on the cathode surface is dif- ﬁcult to convert to the soluble LiPSs, due to the high activation energy needed to overcome the nucleation barrier of solid Li2S2/ Li2S. The irreversible conversion of Li2S2/Li2S further reduces the utilization of the active materials for both cathode and anode, andﬁnally results in the dramatical capacity decay.
Although polar host materials can adsorb the LiPSs, they only mitigate the shuttle effect to some extent. The limited active adsorption sites of the polar materials are difﬁcult to capture the continuously generated LiPSs, leading to the saturation of LiPSs. Moreover, the utilization of sulfur and the redox reaction kinetics of LiPSs are yet to be improved by these polar adsorbents. The catalytic materials, in contrast, do not only capture the LiPSs with their active sites, but also enhance the redox reaction kinetics by accelerating the ion/electron transport.
Figure 1. a) The typical charge/discharge proﬁles for Li–S batteries. Reproduced with permission.[17c]Copyright 2017, Wiley-VCH. b) Schematic illustra- tion of nitrogen-doped CNT/MoS2nanosheets architecture for chemically immobilizing LiPSs and catalyzing the conversion of lithium polysulﬁdes (LiPSs). Reproduced with permission.Copyright 2019, The Royal Society of Chemistry.
Especially, the conversion rate between the soluble LiPSs and the insoluble Li2S2/Li2S can be enhanced. Thereby, the catalytic materials can effectively alleviate the shuttle effect and improve the utilization of active sulfur.
To date, a variety of catalytic materials have been developed for Li–S batteries, including metal-free materials and metal-based materials.[15a,e,21] Metal-free catalytic materials are promising for Li–S batteries due to their low cost and light weight, which are beneﬁcial for gravimetric energy density. Typically, N-doped carbon was reported as a Lewis base catalyst, the lone pair elec- trons of pyridinic and pyrrolic N have strong interactions with LiPSs and can accelerate the conversion of LiPSs. Carbon nitrides are used for Li–S batteries owing to their chemical sta- bility and unique structure, such as the graphitic carbon nitride (g-C3N4).Black phosphorous is another metal-free catalytic material for Li–S batteries, because of its low resistivity, high room-temperature hole mobility, good conductivity, and high binding energies with LiPSs, which can chemically bind LiPSs and convert them to Li2S.Compared to metal-free cat- alytic materials, metal-based catalytic materials have higher electron conductivity and unique electronic properties, which can effectively inhibit the shuttle effect and prolong the electro- chemical performance. The noble metal Pt coated on the Al foil current collector was used as electrocatalytic for Li–S batteries for theﬁrst time,besides, non-noble metals Fe-, Co-, and Ni- based metal catalysts were also reported in Li–S batteries.[21b,26]
Importantly, Fe-, Co-, and Ni-based single-atom catalysts (SACs) are well studied for Li–S batteries in recent years, SAC has unsaturated coordination environment, and atomic-level size which can realize the maximum exposure of the catalytic active sites with 100% utilization efﬁciency (in theoretical). Moreover, transition metal compounds (MaXb, M: metal, X: anion) are one of the largest families of catalytic materials for Li–S batteries because of their unique physical/chemical properties depending on M and X, including oxides, sulﬁdes, and nitridesInterestingly, defect and heter- ostructure can regulate the properties of the catalytic materials and combine different materials as well as their merits, which are widely reported in both metal-free and metal-based catalytic materials.
3. Molybdenum-Based Catalyst Materials for Advanced Li–S Batteries
Molybdenum is a transition metal with an atomic number of 42 and electronegativity of 2.16 on the Pauling scale.In its pure form, Mo is a silvery-gray metal, and can form a variety of chemical compounds in oxidation states fromII toþIV.
Mo-bearing enzymes are by far the most common bacterial cata- lysts for breaking the chemical bond in atmospheric molecular nitrogen in the process of biological nitrogenﬁxation. Mo- based compounds are also widely used in the electrochemical water splitting towards hydrogen evolution reaction (HER),
and have been considered as a promising alternative for HER due to their Pt-like activity and low cost.Recently, Mo-based catalytic materials have been reported as highly efﬁcient catalysts for advanced Li–S batteries (Figure 2).
3.1. Molybdenum Sulﬁdes 3.1.1. MoS2Nanosheets
Arava and coworkers reported the catalytic effect of atomically thin monolayer/few-layer MoS2. Today, MoS2-based compo- sites have been widely studied as effective sulfur host materials for Li–S batteries, because of their highly efﬁcient LiPSs catalytic activity. Monolayer/few-layer MoS2 nanosheets can be pre- pared by chemical vapor deposition (CVD) and shear-exfoliation methods at large scales. They facilitate electron transfer in the transformation reaction, which is initiated by the spatially local- ized adsorption of LiPSs by the unsaturated sulfur atoms at the edge sites (Figure 3a). Interestingly, the X-ray photoelectron spectroscopy (XPS) peaks related to the sulfate complexes are diminished after full discharge, accompanied by the increased intensity of short-chain LiPSs peaks and the slightly lowered binding energy.
Ling and coworkers integrated few-layer MoS2, active sulfur, and conductive reduced graphene oxide (rGO) into a hybrid sul- fur cathode system (MoS2/S/rGO). During the electrochemical process, MoS2nanosheets act as a multifunctional electrocata- lyst. They can chemically adsorb LiPSs and, at the same time, kinetically accelerate the sulfur redox reactions.With theoret- ical calculations, it is shown that MoS2nanosheets can reduce the Gibbs free energy for the rate-limiting step of sulfur reduction and the dissociation energy of Li2S (Figure 3b).
When MHCS@MoS2 (mesoporous hollow carbon sphere coated with MoS2 nanosheets) is used as the sulfur host, the reduction of sulfur and the oxidation of Li2S can be signiﬁcantly accelerated, contributing to suppressed shuttle effect of LiPSs and prolonged lifespan. Thus, the MHCS@MoS2/S cathode showed an ultralow capacity decay of 0.05% per cycle after 500 cycles at 1.0C.
High-loading Li–S batteries using ultrathin MoS2nanosheets catalyst were also reported by Li and coworkers.MoS2nano- sheets were uniformly assembled in the carbon framework Figure 2. Varieties of Mo-based catalytic materials used for Li–S batteries, including Mo sulﬁdes, diselenides, carbides, nitrides, oxides, phosphides, borides, and metal/single atoms/clusters.
(C@MoS2). The good interface compatibility between the 2D conductive and catalytic building blocks enables a built-in catalytic conversion reaction in Li–S batteries (Figure 3c). This catalyst-in-conductor design enables a high sulfur loading of close to 80 wt%, and high capacity/cycling sustainability under a high sulfur loading of 6.0 mg cm2. Similarly, high sulfur mass loading and high volumetric capacity were achieved by Zhang and coworkers. They used the rGo decorated with metallic 1T-MoS2nanoﬂowers (FM@C) as the sulfur host. The S-deﬁcient metallic MoS2nanoﬂowers in FM@G nanosheet process abun- dant accessible catalytic surface and fast electron transfer for chemical adsorption/catalytic conversion of LiPS. Thus, a high volumetric capacity of 1360 mAh cm3 at 4.27 mA cm2 was achieved in an ultrahigh sulfur mass loading up to 87 wt%
(5.1 mg cm2) (Figure 3d).
In addition, MoS2nanosheets are also widely used as separa- tor coating materials or interlayers to suppress the shuttle effect through their chemical interactions with the LiPSs.For exam- ple, Tang et al. prepared theﬂexible MoS2/Celgard composite separator using the simple ﬁltration method (Figure 4a).
When used as a separator in Li–S batteries, it can prevent LiPSs diffusion, thus signiﬁcantly suppressing the LiPSs shut- tling and yielding high Coulombic efﬁciency. Moreover, because of the excellent Li ion conductivity of the composite separator, it can facilitate the transport of Li ions and improve the lifespan and rate capability of Li–S batteries. Xie et al. fabricated a dual-functional separator coated by layer-by-layer self-assembled few-layer MoS2and polymer (Figure 4b). When only coated 0.1 mg cm2, the Li–S batteries show excellent cycle stability with a negligible capacity decay of 0.029% per cycle over 2000 cycles at Figure 3. MoS2nanosheets used as effective sulfur host materials for Li–S batteries. a) Schematic illustration of transition metal dichalcogenide (MoS2) nanosheets for LiS battery, showing conﬁned deposition of LiPSs at preferential catalytic sites and their conversions during discharge–charge proc- essing. Optical and scanning electron microscope (SEM) images of MoS2ﬂakes before and after deposition of LiPSs, and elemental mapping of sulfur.
Reproduced with permission.Copyright 2016, American Chemical Society. b) Energy proﬁles for the sulfur reduction on carbon and MoS2substrates, and energy proﬁles of the decomposition of Li2S cluster. Reproduced with permission.Copyright 2020, Elsevier. c) Illustration of conﬁned nanoreactors in porous cavities between 2D (conductive) carbon layers with internal faces decorated by 2D (catalytic) MoS2nanosheets. Reproduced with permis- sion.Copyright 2020, American Chemical Society. d) Schematic illustration for the synthesis of FM@G and the systematic effect of a Li–S battery cycling performance at 0.5 and 1.0C. Reproduced with permission.Copyright 2021, Wiley-VCH.
1C, an enhanced rate capability of 766 mAh g1at 3C, and a large reversible areal capability of 2.0 mAh cm1at 1C over 400 cycles.
To further improve the electrical conductivity during the elec- trochemical process, MoS2 nanosheets combined with highly conductive carbon composites were used as the interlayer for Li–S batteries.Wang et al. developed MoS2/carbon nanotubes (CNT) interlayer by uniformly loading nanosheets on a cross- stacked CNTﬁlm (Figure 4c).The CNTﬁlm provided good electrical conductivity for the sulfur cathode and a supporting skeleton for the dispersion of MoS2, which further suppressed the shuttle effect through their chemical interactions with the LiPSs. The MoS2 nanosheets encapsulated by nitrogen- doped carbon (MoS2/NC) are also used as the interlayer (Figure 4d). The homogeneous core–shell design ensures the intimate contact between MoS2 and carbon, providing a smooth ﬂow of electrons through the entire interlayer system to accelerate the LiPSs conversion. Therefore, highly efﬁcient LiPSs immobilization and fast LiPSs kinetics can be realized, leading to an outstanding cyclability over 1500 cycles (with only 0.034% fading per cycle), improved rate performance, and high areal capacities of up to 3.7 mAh cm2. Interestingly, Zhang et al.
designed a layer-spacing-enlarged MoS2(LE-MoS2) consisting of
hierarchical superstructural nanosheets for Li–S batteries (Figure 4e). Due to the expanded (002) lattice plane of MoS2, the catalytic effect on the LiPSs transformation kinetics and the immobilization effect are both enhanced, which were also proved by the in situ X-ray adsorption near-edge structure spectroscopy and ﬁrst-principles calculation. As a result, sulfur-loaded LE-MoS2 shows a high initial capacity of 1550 mAh g1, a low capacity fade rate of 0.06% per cycle, and a long-term lifespan of up to 500 cycles at 1C.
A heterojunction is an interface between two layers or regions of dissimilar semiconductors, and a heterostructure contains mul- tiple heterojunctions. Inspired by the unique band structure and synergistic effect of the heterostructure, MoS2-based heterostruc- tures are widely used as a sulfur host in recent years.
Zeng et al. reported the in situ growth of MoS2 on nitrogen, sulfur DCC crosslinked BaMn0.9Mg0.1O3 perovskite particle (PrNP), and CNTs heterostructure (DCC@MoS2/PrNP/CNTs) (Figure 5a). The DCC@MoS2/PrNP/CNTs heterostructure displays a perfect 3D interconnected e/Liþ conductive Figure 4.MoS2nanosheets used as separator coating materials or interlayers for Li–S batteries. a) SEM images of MoS2/Celgard surface and cross- section of MoS2layers. Reproduced with permission.Copyright 2017, Wiley-VCH. b) Schematic showing the layer-by-layer self-assembly process of MoS2-polymer modiﬁed separator for Li–S battery. Reproduced with permission.Copyright 2018, Wiley-VCH. c) Schematic diagram of a Li–S cell with the MoS2/CNT interlayer, electrochemical impedance spectroscopy (EIS) spectra of the fresh cells with the MoS2/CNT-interlayer-coated separator and pristine separator. Reproduced with permission.Copyright 2018, Elsevier. d) Rate performance measured from 0.2 to 2C and the cycling stability at 1C after the step-wise rate performance at an increased sulfur loading of 4.0 mg cm2with MoS2nanosheet@N-doped carbon interlayer. Reproduced with permission.Copyright 2019, The Royal Society of Chemistry 2019. e) Schematic illustration of LE-MoS2preparation and its enlarged interlayer. Sulfur K-edge X-ray absorption near edge structure with and without S/LE-MoS2electrode, splitting energy proﬁles for the transition from Li2S4to Li2S.
Reproduced with permission.Copyright 2020, American Chemical Society.
framework and a cooperative interface from amphipathicity sites synergistically bonded with the bipolar head of LiPSs. This struc- ture stimulates the efﬁcient immobilization and rapid conversion of LiPSs. Even with a high sulfur loading of 5.2 mg cm2, the heterostructure electrode still provides a high initial capacity of 882.7 mAh g1and an areal capacity of 4.75 mAh cm2after 50 cycles at 0.2C.
Xu et al. synthesized atomic-scale Co9S8@MoS2 core–shell heterostructure-embedded carbon nanoﬁber (CNF) (Co9S8@MoS2/CNF). The core–shell heterostructure modiﬁes the band structure of MoS2(Figure 5b) and hence its electrical conductivity, leading to the enhancement of the chemical adsorp- tion of LiPSs and the catalytic conversion of LiPSs to Li2S.As a result, the assembled Li–S batteries demonstrated a high discharge speciﬁc capacity of 477 mAh g1 at a high current density of 5C. And even with high sulfur loadings of 6 and
10 mg cm2, high capacities of 1002 and 986 mAh g1 can be obtained after 50 cycles, respectively. Zhang et al. synthesized the MoS2–MoO3heterostructure and modiﬁed the separator for Li–S batteries. These heterostructures can provide high surface area and strong polar surface afﬁnity for trapping LiPSs (Figure 5c). Furthermore, the generated crystal distortions near the interface with more active sites could also promote the redox reaction of LiPSs. As a result, Li–S batteries with the MoS2–MoO3heterostructure show a high initial discharge capac- ity of 1531 mAh g1at 0.2C, and only 0.0135% capacity decay per cycle after 600 cycles at 1C. Even at a high sulfur loading of 5.9 mg cm2, Li–S batteries still deliver a capacity of 640 mAh g1after 100 cycles at 0.2C.
MoS2/nitrogen-doped reduced graphene oxide (MoS2/C) heterogeneous interface can also signiﬁcantly promote the transformation of LiPSs and decomposition of Li2S. The Figure 5. MoS2-based heterostructures used as the sulfur host. a) Schematic illustration of the fabrication process of DCC@MoS2/PrNP/CNTs/S elec- trode. Reproduced with permission.Copyright 2018, Wiley-VCH. b) Schematic illustration of the Co9S8@MoS2/CNF interlayer working in Li–S bat- teries, calculated band structures of MoS2, Co9S8, and Co9S8@MoS2. Reproduced with permission.Copyright 2021, American Chemical Society.
c) Polysulﬁde diffusion tests and the DME/DOL electrolyte contact angle shots of the PP, CS–PP, MoO3/CS–PP, MoS2/CS–PP, and MoS2–MoO3/ CS–PP. Reproduced with permission. Copyright 2020, American Chemical Society. d) XPS spectra of Mo 3dbefore and after adsorption with Li2S6, charge curves at 2.4 V of a Li2S8/tetraglyme solution on different the surfaces, cycling performance under 0 °C, and with high sulfur content.
Reproduced with permission.Copyright 2022, Wiley-VCH.
XPS characteristic peaks of Mo6þdecreased in their intensities, and several Mo 3dpeaks showed a slight shift after the adsorption of Li2S6, indicating a strong chemical reaction between Mo6þand Li2S6. Moreover, compared with the other two electrodes (pure PP separator and nitrogen-doped reduced graphene oxide coated separator), the oxidation of solid Li2S by MoS2/C also exhibited a stronger enhancement, suggesting a signiﬁcantly lower oxidation overpotential for Li2S conversion (Figure 5d). Therefore, the cath- ode with MoS2/C can deliver a high reversible capacity even at the low temperature of 0 °C, and an extremely high areal capacity of 6.11 mAh cm2can be achieved with high sulfur mass loading of 8.0 mg cm2.
3.1.3. Defect-Rich MoS2
Defect engineering is an important strategy to regulate the atomic distribution and optimize the electronic structure of
the nanomaterials, including vacancy and doping. Very recently, defect engineering has been widely used in the modiﬁ- cation of MoS2-based hosts for Li–S batteries, which showed very motivating improvements in the electrochemical performances of these host materials. For instance, Yu et al. developed a 3D graphene aerogel (GA) decorated with defect-rich (vacancy) MoS2 nanosheets (GA-DR-MoS2) as a sulfur host (Figure 6a).During the self-assembly process, the MoS2pre- cursors were adsorbed by the functional groups of GO sheets, meanwhile, an excess of thiourea acts as a reductant for the Mo6þMo4þreaction. In addition, they also serve as an efﬁcient additive for MoS2 nanosheet defect manufacturing. Primary nanocrystallites adsorb excessive thiourea on their surface, thus partially impeding oriented crystal growth and forming a defect- rich structure. When used as an electrocatalyst for Li–S batteries, the defect-rich MoS2 can signiﬁcantly accelerate LiPSs redox kinetics during the electrochemical process owing to the
Figure 6. Defect-rich MoS2used for Li–S batteries. a) Schematic illustration of the GA-DR-MoS2/S composite fabrication process. Reproduced with permission.Copyright 2019, American Chemical Society. b) Schematic illustration of the defect-rich MoS2/NC composite construction process and the working mechanism in Li–S batteries. Reproduced with permission.Copyright 2020, American Chemical Society. c) Schematic of the structure and phase transition of MoS2after Co-doping, Li2S4and Li2S decomposition energies on 1T MoS2and 1T Co–MoS2monolayer. Reproduced with permission.Copyright 2021, American Chemical Society. d) Density of states (DOS) plots for MoS2and P–MoS2, and partial density of states (PDOS) results of P–MoS2. Reproduced with permission.Copyright 2021, Elsevier. e) Electron localization function (ELF) plots of the MoS2–B–
S8adsorption system and the MoS2–B–Li2S4adsorption system; schematic for Lewis acid–base interaction; DOS projected onto Pz orbitals for the MoS2–B–S8adsorption system and the MoS2–B–Li2S4adsorption system; schematic for the sp3hybridization of B in MoS2–B and the head-on orbital overlap between B and S. Reproduced with permission.Copyright 2021, American Chemical Society.
enhanced exposure of active edge sites. Similarly, the defect-rich MoS2/N-doped carbon nanosheets (MoS2/NC) were synthesized by the aforementioned method (Shen et al. Figure 6b), and the obtained composite-coated PP (MoS2/NC@PP) separator was used as a modiﬁed separator for Li–S batteries.This modiﬁed separator demonstrated multifunctional effects: 1) the N-doped porous carbon nanosheets can be used as a conductive network to ensure fast electron transfer; 2) The defect-rich MoS2can not only effectively capture LiPSs and suppress the shuttle effect, but also offer abundant catalytic activity sites to enable fast redox reaction kinetics.
Heteroatom doping is another approach to tailor the electric conductivity, electronic conﬁguration, and surface property of the nanomaterials, which can further tune the catalytic activity of the host materials for Li–S batteries. Lv et al. prepared a Co-doped MoS2 (Co–MoS2) through a hydrothermal method (Figure 6c), the density-functional theory (DFT) calculation suggests that the introduction of Co atoms can help to stabilize the 1T MoS2, and the sulfur vacancy formation energy also decreases from 3.38 eV (2H MoS2) to 1.92 eV (1T Co-doped MoS2).
Moreover, The Li2S4, Li2S2, and Li2S decomposition energies on 1T MoS2are 2.842, 2.403, and 2.261 eV, which decrease to 2.384, 1.529, and 1.441 eV after Co-doping, respectively, illustrat- ing the 1T Co–MoS2has much better catalytic activity toward the redox reaction of LiPSs. In addition, non-metallic P element dop- ing MoS2 (P–MoS2) was reported to modify the separator by Zhao et al. (Figure 6d), from the DFT calculation, the electronic states and new defect levels occur in P–MoS2 com- pared to that of the pristine MoS2at the Fermi level. And the partial density of states (PDOS) reveals that the P 2p orbital has strong hybridization with its neighboring Mo 3d orbital and S 2p orbital at the Fermi level. These results show that the introduction of P doped in MoS2leads to more charge trans- fers and increases the conductivity of MoS2. In addition, the bond length of Li–S on the surface of P–MoS2is also the longest com- pared with MoS2and pristine Li2S during the charging process, (2.399, 2.270, and 2.099 Å, respectively). A longer bond length helps to weaken the bond between atoms, thereby promoting the conversion of LiPSs and accelerating the redox kinetics.
Interestingly, B-doping was reported by Zhao et al. to tune the orbital orientation of MoS2. From the electron localization function (ELF) analysis, there are two electron localized areas around each S atom in S8 (Figure 6e), which represent the two lone pairs of electrons, and one lone pair of electrons is used to form B–S coordinate link between MoS2–B and S8. In addi- tion, MoS2–B can also form B─S covalent bonding with Li2S4. The highest occupied molecular orbital (HOMO) of S (Lewis base) interacts with the lowest unoccupied molecular orbital (LUMO) of B (Lewis acid) to give a Lewis acid–base complex.
Their interaction produces a coordinate covalent bond where S donates an electron pair to B. The DOS projected onto Pz orbi- tals for the MoS2–B–S8 and the MoS2–B–Li2S4adsorption sys- tems. The signiﬁcant electronic state overlap of Pz orbitals between B and S provides strong evidence for their intensive z-directional orbital coupling. The perpendicular orientation of the vacant orbital of B allows for maximal head-on overlap (σ bonding) with the occupied orbital of S to form a stable B─S bond. Thus, the basal plane of MoS2 is efﬁciently activated;
the CNT@MoS2–B catalyst exhibits outstanding catalytic activity
toward sulfur redox reactions, and achieves superior electro- chemical performances for Li–S batteries.
For MoS2, with its comparatively facile and controllable syn- thesis (of derivatives), including MoS2nanosheets, MoS2heter- ostructure, and defect-rich MoS2, plenty of works suggest they can display enhanced electrochemical interactions with LiPSs, which are greatly promoting the catalytic materials for Li–S bat- teries. However, there is still room to further improve the activity of MoS2catalysts, for instance, 1) downsizing and maximizing the number of active sites; 2) using the few-layer or even single-layer MoS2nanosheets; 3) improving the intrinsic activity by tuning the electronic structure.
3.2. Molybdenum Diselenides/Tellurides
As isomorphic to MoS2, the bandgap reduces when the chalco- gen changes from S to Te, and the total density of states in the vicinity of the Fermi level for MoSe2 and MoTe2, conforming their metallic character and higher conductivity than MoS2, which will potentially promote faster electrocatalyst activity to LiPSs, even though they have attracted much less attention than MoS2so far. Zhang et al. integrated MoSe2nanoﬂakes with car- bon nanotube, and coated them on the PP separator for Li–S bat- teries (MoSe2/CNT-PP) (Figure 7a).Due to the polar nature of the MoSe2nanoﬂakes, strong chemisorption can be provided for LiPSs, and the CNTs can work as a charge transport channel.
Li–S batteries with MoSe2/CNT–PP separator deliver higher ini- tial capacity, much better rate performance and cycling stability.
Moreover, MoSe2-based heterostructure and heteroatom dop- ing were also investigated as sulfur hosts. For example, Liu et al.
prepared the MoSe2@FC@Mo2C heterostructure in which tran- sition metal MoSe2and metallic Mo2C are encapsulated into hol- low ﬂuorine co-doped carbon materials (Figure 7b).
Interestingly, when the MoSe2@FC@Mo2C heterostructure was used for Li–S batteries, the MoSe2, Mo2C, and FC demon- strated synergistic electrocatalysis activity, and the polar FC with strong electronegativity tend to promote the conversion of long- chain (S8 ↔ Li2S4), while the polar MoSe2 and Mo2C with enriched oxygen vacancies accelerate the short-chain conversion (Li2S4↔Li2S). Thus, leading to fast redox kinetics of LiPSs, and displaying good performance even under a high sulfur contenting of 5.5 mg cm2 and a lean E/S ratio of 5 mL g1. Similarly, Zhang et al. synthesized the MoSe2/MoO2heterostruc- ture by water-steam etching and used as the sulfur host (Figure 7c).The MoSe2/MoO2heterostructure can accelerate ionic diffusion and enhance electrolyte accessibility due to the excellent conductivity of MoSe2. Moreover, the synergistic cata- lytic behavior and efﬁcient trapping and conversion of LiPSs can be realized by the formation of the heterostructure.
Li et al. designed a bifunctional electrocatalyst by the manip- ulation of cation cobalt doping into MoSe2(Co–MoSe2), which is in situ hybridized with conductive MXene nanosheets via a one- step hydrothermal reaction. In this design, cobalt doping is used to tailor the electronic structure and reactive sites of MoSe2to enhance the intrinsic catalytic activity and conductivity of MoSe2.From the cyclic voltammetry (CV) of symmetric cells, a higher current density was displayed for Co–MoSe2/MXene (1.8 A g1) compared to that of pure MoSe2/MXene
(1.25 A g1), suggesting that the catalytic conversion ability was signiﬁcantly improved after Co doping. Impressively, even with the resultant dense S/Co–MoSe2/MXene monolith cathode (13.5 mg cm2), the Li–S battery still delivered a high initial gravimetric capacity of 1454 mAh g1and an ultrahigh volumet- ric energy density of 3659 Wh L1at 0.1C (Figure 7d). Sun et al.
proposed the introduction of N-doping (DN) and Se-vacancies (VSe) in the MoSe2electrocatalyst for sulfur chemistry.The CV proﬁles reveal that the S@N–MoSe2x/C electrode displayed the largest current response and the lowest reaction polarization
for all redox peaks, suggesting expedited sulfur redox kinetics originating from dual-defect engineering. Importantly,DN sig- niﬁcantly decreased the Tafel slope, while further incorporation ofVSecritically decreased. Since a smaller Tafel slope means a faster electrokinetic process, it could be corroborated thatDNand VSe selectively accelerate the Li2S nucleation and dissociation reactions, respectively (Figure 7e).
MoTe2with different phases (2H, 1T, and 1T’) were investi- gated to prevent the shuttle effect for Li–S batteries, and the DFT calculations suggested that the 1T’-MoTe2 showed the Figure 7. MoSe2/MoTe2electrocatalyst used for Li–S batteries. a) The preparation process of MoSe2/CNT–PP separator. Digital photos of Li foil, Li foil with M/C–PP, and Li foil with PP. Reproduced with permission. Copyright 2021, Elsevier. b) The schematic diagram for the preparation of MoSe2@FC@Mo2C/S process. Reproduced with permission.Copyright 2020, Elsevier. c) The schematic illustration of the synthesis process of S/MoSe2/MoO2heterostructure. Reproduced with permission.Copyright 2019, Elsevier. d) Areal capacities and cycling stability of a thick and dense monolith cathode and a dense self–supporting monolith cathode at 0.1C. Reproduced with permission.Copyright 2021, American Chemical Society.
e) CV proﬁles of S@N–MoSe2x/C, S@N–MoSe2/C, and S@MoSe2/C electrodes at a scan rate of 0.05 mV s1. Tafel plots of peak ii and peak iii.
Reproduced with permission.Copyright 2021, Wiley-VCH.
concentrated density of states (DOS) close to Fermi level with high conductivity.Moreover, the in situ Raman spectroscopy revealed that the signals of high intensity of different mid- and long-chain (S82, S62, and S42) can be unmistakably distinguished from the time-resolved Raman image for the gra- phene/S cathode, while there are no obvious S82, S62, or S42 Raman shifts noticed for the 1T0-MoTe2based cathode. Owing to the chemisorption and high catalytic effect of 1T0-MoTe2, 1T0- MoTe2-based cathode exhibits a highly reversible discharge capacity of 1310.1 mAh g1 at 0.2C with 0.026% capacity fade rate per cycle over 600 cycles.
MoSe2and MoTe2have similar properties to MoS2, the strate- gies to improve the activities for MoSe2and MoTe2 can learn from MoS2. However, the weight of MoSe2and MoTe2is much heavier than MoS2, the weight ratio of catalytic materials in the cathode needs to be considered when used in Li–S batteries.
3.3. Molybdenum Carbides
Mo carbides (MoxC), with high conductivity, metallic character- istic, and superior catalytic effect are investigated as sulfur cata- lytic materials in recent years.[32,64]Liu et al. reported a uniform hollow structure constructed of double carbon shells and fully embedded polar metallic Mo2C (Mo2C/C@C) as the sulfur
host.Similarly, Lai et al. synthesized a hierarchical defective MoxC@N-doped carbon hollow microsphere (MoxC@NC) used for Li–S batteries.The hierarchical hollow structure can facili- tate electrolyte inﬁltration and fast electron/ion transportation, and buffer the volumetric expansion during the electrochemical process. Moreover, the defective MoxC with enhanced electro- chemical interaction with LiPSs (Figure 8a), thus, the S cathode with MoxC@NC catalyst delivered a favorable speciﬁc capacity of 982 mAh g1at 0.5C, and maintained over 400 cycles with a low- capacity fading rate of 0.14% per cycle.
Interestingly, Qi et al. reported a Ni-tipped CNTs-on-MoC porous pillar foundation (MoC@NiNCNT) hierarchical nano- reactor with multiadsorption-catalytic sites produced by the CVD process (Figure 8b).First, the dicyandiamide released the vol- atile CNx gas when the calcination temperature reached at 600 °C, which is trapped by NiMoO4 nanorods, triggering the exsolution of Ni nanoparticles and promoting the NiMoO4trans- formed into Ni/MoOxto form MoN. Finally, the MoN converted to the MoC with a large number of nanoscale pores when the temperature reached 800 °C. Beneﬁting from these favorable fea- tures, even under a high sulfur loading of 6 mg cm2, Li–S bat- teries with MoC@NiNCNT catalyst can achieve a large areal capacity of 6.1 mAh cm2at 0.5C.
Since the small size of catalysts will provide more active sites, many efforts have been devoted to optimizing the
Figure 8. MoCx-based electrocatalyst used for Li–S batteries. a) Enhanced electrochemical interaction between MoxC and LiPSs. Reproduced with per- mission.Copyright 2022, The Royal Society of Chemistry. b) Schematic illustration of the direct chemical vapor deposition (CVD) fabrication of MoC@NiNCNT on the CFC substrate. Reproduced with permission from .Copyright 2021, American Chemical Society. c) The Mo2C quantum dots homogeneously anchor on graphene nanosheets. Reproduced with permission from .Copyright 2020, Elsevier. d) SEM image and corresponding elemental maps of S, Mo, C, O and F, EDS spectra after 50 cycles, and long-term cycling performance at the rate of 1C for 600 cycles. Reproduced with permission.Copyright 2020, Elsevier.
size/morphology of the MoxC-based catalysts. He et al.
reported a novel Mo2C quantum dots@graphene functionalized separator for Li–S batteries.The precursor gel of Mo2C quan- tum dots (QDs) anchored N-doped graphene (NG) nanosheets (P-MQD@NG) was synthesized by hydrothermal method, then (NH4)6Mo7O24·4H2O and poly(oxypropylene) diamines (D400) was dissolved into graphene oxide solution, the P-MQD@NG was obtained when heating the solution at 90 °C. After freeze- drying, the MQD@NG can be obtained by annealing in an Ar atmosphere. Signiﬁcantly, the high-resolution transmission elec- tron microscopy (HRTEM) image strongly supports the Mo2C quantum dots homogeneously anchor on graphene nanosheets, and have a uniform morphology with an average diameter of only 1.8 nm (Figure 8c). Liu et al. prepared the ultraﬁne Mo2C nano- crystallites encapsulated in porous carbon substrate (Mo2C– CNOs) via a MOFs-assisted strategy.When used as the sulfur host for Li–S batteries, the highly polar Mo2C can chemically adsorb the LiPSs due to the formation of a strong Mo─S bond.
Besides, the Mo2C nanoparticles with enhanced electrocatalytic activity can boost the redox reaction kinetics of sulfur species dur- ing the electrochemical process. As a result, even with a high sul- fur content of 72.15 wt%, the S cathode with Mo2C–CNOs catalyst can deliver a favorable speciﬁc capacity of 1396 mAh g1at 0.1C.
Similarly, Li et al. reported the Ketjenblack matrix decorated with ultra-small Mo2C nanoparticles (KB/US-Mo2C) by“in situ growth” strategy, and coated on the PP separator for Li–S batteries.
Compared to the traditional S cathode slurry coating process, S electrodes with a freestanding structure can avoid the inactive components, such as, binders, conductive agents, and alumin- ium current collectors, thus, improving the energy density of the Li–S batteries. Lu et al. fabricated freestanding Mo2C- decorated N-doping carbon nanoﬁbers (Mo2C-NCNFs) as a 3D current collector for Li–S batteries. This interconnected 3D nanoﬁbers structure guarantees structural integrity, excellent elec- tronic transport, and fast electrochemical reaction kinetics.
Cheng et al. reported the graphene@Mo2C nanoparticles (GCF- G@Mo2C) heterostructure supported by lightweight graphitic carbon foam as the freestanding S electrode for Li–S batteries (Figure 8d).The N-doped carbon foam wrapped by graphene sheets with an agaric-like porous structure can achieve fast mass transport and electrolyte inﬁltration, and high S mass loading.
When combined with Mo2C electrocatalyst, it can afford effective anchoring/catalytic sites to LiPSs. As a result, this architecture of GCF-G@Mo2C can accommodate extremely high sulfur loading up to 10.5 mg cm2, exceeding most of the previous Li–S works.
For Mo carbides, they show high conductivity, metallic char- acteristic, and enhanced catalytic effect for LiPSs, nevertheless, high-temperature conditions are required during the synthesis, and the well-deﬁned crystalline phase is often difﬁcult to obtain.
Therefore, more controllable synthesis approaches with moder- ate temperatures should be developed for MoCxcatalysts.
3.4. Molybdenum Nitrides
Mo nitrides with a polar structure and high electrical conductivity have been widely investigated as the sulfur hosts for Li–S batter- ies.Wang et al. reported the template-assisted fabrication of mesoporous and conductive Mo2N with a high surface area of
121 m2g1, a pore size of 8.6 nm, and a conductivity of 1105S m1(Figure 9a). During the electrochemical process, conductive interwoven skeletons can speed up electron transport, and boost LiPSs redox conversion. In addition, mesoporous Mo2N with a high surface area provides a high polar surface area for chemical binding LiPSs and efﬁcient suppression shuttling effect.Similarly, Sun et al. fabricated the MoN microrod using the one-pot ammoniation strategy of the metal–oxide template, even with a high areal loading of 3.1 mg cm2, the MoN–S cath- ode could deliver an initial discharge capacity of 1315 mAh g1 and maintain a reversible capacity of 902 mAh g1 after 350 cycles.Liang et al. prepared thorn-like carbon nanoﬁbers combined with MoN nanosheets (MoN@CNFs). Using the MoN as a multifunctional coating to modify conventional Celgard sep- arators, Li–S batteries can achieve impressive performance because the MoN nanosheets can chemically anchor polysulﬁdes and distinctly improve the redox kinetics of LiPSs (Figure 9b).
The heterostructural mediators combining high conductivity and high polarity can accelerate the LiPSs conversion and regu- late the deposition of solid Li2S/Li2S2.Recently, MoN/Mo2N- based heterostructures were reported for Li–S batteries, Cao et al.
designed the MoO2–Mo2N nanobelts as the multifunctional interlayer for Li–S batteries (Figure 9c).After interacting with Li2S6, the valence state of Mo from the MoO2sample showed slight binding energy shifts around0.5–0.8 eV, which indi- cates the electron exchange between Li2S6. And a new peak around 529.48 eV in MoO2–Li2S6 represents the formation of Li–O binding after the chemisorption to Li2S6 species and MoO2. Similarly, a certain amount of Mo6þin Mo2N was reduced and the peaks of both Mo4þ, Mo5þ, and Moδþshifted to lower binding energy owing to the increased electron density at the metal center. And a negative shift of the Mo–N peak (from 394.82 to 394.19 eV) also indicates the interaction between Li- ion and N atom. These XPS results demonstrate that the MoO2–Mo2N binary structure can sufﬁciently restrict the shut- tling of LiPSs and prompt the conversion kinetics. Sun et al.
designed the MoS2–MoN heterostructure nanosheets as sulfur hosts.From the hard X-ray micro-analysis (HXMA), the Mo pre-edge in the MoS2host moves slightly to a lower energy posi- tion. On the contrary, the Mo pre-edges in MoS2–MoN and MoN hosts shift to higher energy positions, indicating that the valance of Mo ions ascends after reaction with Li2S6.Because of their respective advantages, LiPSs trapping ability and fast surface Liþ diffusion (by MoS2) as well as high electron conductivity and cou- pled electron transfer through redox reaction (by MoN) for LiPS conversion, the MoS2–MoN host could show high areal capacity even with ultrahigh loadings of 12.2 mg cm2(sulfur content of 72.7%) and lean electrolyte usage down to 4.2 mL g1.
Mo nitrides have high conductivity, polar structure, and enhanced catalytic properties, which can anchor LiPSs and accel- erate sulfur redox kinetics. However, similar to Mo carbides, the synthesis of Mo nitrides generally needs high-temperature con- ditions and lack a facile synthesis approach.
3.5. Molybdenum Oxides
Mo oxides are a kind of polar metal oxides with high electronic conductivity, wide bandgap, and abundant oxygen vacancies,
which exhibit versatile catalytic activities for many reactions.
Xiang et al. synthesized the reduced graphene oxide/
molybdenum dioxide (rGO/MoO2) composite to modify the PP separator for Li–S batteries.The modiﬁed PP separator introduces physical adsorption, chemical anchoring, and cata- lytic effects to restrain the“shuttle effect”, thus improving the electrochemical performances of Li–S batteries. MoO3 nano- particlesand MoO3sphereswere also used for Li–S bat- teries, the layer structure of MoO3with octahedral holes and extension channels, which can function as the embedding loca- tions and diffusing channels for Liþ, and the oxygen atoms on the MoO3host can form the chemical binding interactions with LiPSs, thus alleviating the dissolution of the LiPSs (Figure 10a).
In addition, Zhao et al. reported the growth of MoO3 nano- ﬂakes onto the carbon paper (MoO3-CP), which served as an efﬁcient cathode electrode for Li–S batteries.Because the MoO3 can offer a strong binding ability to anchor LiPSs at the electrode surface and exhibit extraordinary catalytic activity toward LiPSs redox reaction, even with a high sulfur loading of 8 mg cm2, the speciﬁc capacity retention rate of Li–S batteries can still keep as high as 68.75% after 1000 cycles at 1C (Figure 10b).
MoO2-based heterostructures were also used for Li–S batter- ies, for instance, Manthiram et al. reported the in situ growth of the MoO2/MoS2 hybrid nanosheets onto the carbon cloth (MoO2/MoS2@CC),the MoO2/MoS2hybrid integrates the advantages of conductive MoO2 and sulﬁphilic MoS2, which exhibits excellent catalytic effect, enhances charge transfer and greatly promotes the redox kinetics of LiPSs
transformation. As shown in Figure 10c, the CV curves with MoO2/MoS2 nanosheets have much sharper peaks, lower polarization, and lower redox peak separation between cathodic and anodic peaks, illustrating the enhanced redox kinetics.
Besides, the Nyquist plots revealed a lower resistance com- pared with the pure carbon paper, implying the great enhance- ment in charge transfer brought by MoO2/MoS2nanosheets.
The insulating Li2S layer may lead to rapid passivation of the surface during the electrochemical process and result in poor reaction kinetics, thus impeding the subsequent Li2S deposition and resulting the fast capacity decay. Cao et al.
reported that the MoO2/α-MoC heterostructure can inﬂuence the redox process of sulfur species and Li2S deposition behavior. The capacity of Li2S is 160, 167, and 245 mAh g1 when precipitation on MoO2, α-MoC, and MoO2/α-MoC, respectively, indicating that MoO2/α-MoC is conducive to facilitating the liquid–solid phase transformation (Li2S4–Li2S) during the electrochemical process (Figure 10d).
Moreover, the oxidation response current of the MoO2/α- MoC electrode is higher than MoO2 and α-MoC electrodes, suggesting improved catalytic activity of the MoO2/α-MoC heterostructure.
Polar Mo oxides with low cost, wide bandgap, and abundant oxygen vacancies on the surface, which exhibit versatile cata- lytic activities for LiPSs, while the electrical conductivity of Mo oxides is relatively low, the tuning of electron structure and/or introducing of conductive frameworks for Mo oxides are highly necessary.
Figure 9. Mo nitrides used as sulfur host materials. a) Schematic illustration of the fabrication of mesoporous-Mo2N. Reproduced with permission.
Copyright 2018, Elsevier. b) The LiPSs anchoring and enhanced conversion on the surface of exposed MoN nanosheets. Reproduced with permission.
Copyright 2022. American Chemical Society. c) The synergistic catalytic conversion of LiPSs by the MoS2–MoN heterostructure, hard X-ray micro-analysis (HXMA) spectra of molybdenum K-edge before/after soaking in Li2S6solutions, and long-term cycling performance. Reproduced with permission.
Copyright 2021, Wiley-VCH.
3.6. Other Mo-Based Compounds
Mo phosphides have high electron conductivity and strong inter- action with LiPSs, which are investigated for Li–S batteries.
Li et al. synthesized the Ru-doped Mo4P3 nanoparticles and employed it as sulfur hosts (Figure 11a).The Ru 3pXPS spec- trum showed that a new peak observed at 482.6 eV can be assigned to the Ru─S bond after immersion with Li2S4, revealing the strong interaction of Ru with LiPS; at meaning while, the Mo 3d5/2and 3d3/2peaks of Mo 3dspectra shifted to the lower bind- ing energy of 232.1 and 228.0 eV, reﬂecting the interaction of Mo with LiPSs. Thus, the Ru–Mo4P3 electrode delivered excellent rate capability with a capacity of 660 mAh g1 at 4C, and a low-capacity decay of 0.07% per cycle at 3C even with a high S content of 77%. Moreover, Chen et al. reported the MoP quantum dots anchored to N, P-doped graphene (MPQ@G) as a highly efﬁ- cient electrocatalyst for Li–S batteries (Figure 11b).The MoP quantum dots possess a uniform morphology with an average diameter of 1.6 nm, which provided an abundance of the exposed active sites for LiPSs during the electrochemical process.
In addition, due to the unique advantages of MoP and MoS2, the MoP–MoS2heterostructure was also investigated to modify the PP separator for Li–S batteries (Figure 11c).Theseﬂower-like heterostructures, composed of stacked nanosheets, provide numerous activity sites for LiPSs, thus promoting the reaction kinetics of LiPSs.
Recently, the anchoring and electrocatalysis of Mo borides were extensively studied for Li–S batteries by density functional theory,as shown in Figure 11d, the catalytic performance on the discharge reactions was evaluated by calculating the Gibbs free energy diagrams of S8 and a series LiPSs on Mo2B2O2 and Mo2B2F2. The reduction of S8 to Li2S8on both Mo2B2O2
and Mo2B2F2is exothermic with remarkable energy downhills
of 5.325 and 3.055 eV, respectively, suggesting fast kinetics.
Moreover, the reduction from Li2S2to Li2S has an energy uphill of 0.744 eV on Mo2B2F2, while the free energy has a favorable downhill of 0.322 eV on Mo2B2O2, revealing the S atom of Li2S is adsorbed on the surface of Mo2B2O2. Besides, both Mo2B2O2 and Mo2B2F2 can signiﬁcantly decrease the Li2S decomposition barrier from 3.39 to 1.152/0.441 eV, respectively.
This work provided a general design principle for improving the electrochemical performance of Mo borides for Li–S batteries.
Mo phosphides have similar metallic properties to Mo car- bides, except that phosphorus (P) has a much lower electronega- tivity than that of carbon, which allows Mo phosphides to more efﬁciently catalyze LiPSs conversion. In turn, oxide coating more readily occurs on Mo phosphides surface than on Mo carbides, thus, surface protection for Mo phosphides catalytic materials should be considered.
3.7. Mo-Based Metal/Single Atoms/Cluster
Recently, our group prepared the monodisperse Mo nanopar- ticles with an average diameter of 1.24 nm (embedded onto nitrogen-doped graphene, Mo@N-G) and used as a highly efﬁ- cient catalyst for Li–S batteries (Figure 12a).During the elec- trochemical process, the unﬁlled d orbitals of oxidized Mo can attract electrons from the LiPS anions and form the Mo─S bond, thus promoting the conversion of LiPSs. Importantly, even with only 9% catalyst, the Li–S batteries can exhibit a large initial dis- charge capacity of 1359 mAh g1, superior cycling stability with 92.7% capacity retention over 100 cycles, and enhanced reaction kinetics under large current densities (676 mAh g1, 10C).
Tan et al. fabricated a Mo–Li2S–graphene capsule, where Mo nanocrystal catalysts and graphene-encapsulated shells are Figure 10.Mo oxides used for Li–S batteries. a) Charge density plots of pureα-MoO3c),α-MoO3/Li2S4d) andα-MoO3/Li2S6. Reproduced with per- mission.Copyright 2018, Elsevier. b) The cycling performance of Li–S batteries with MoO3–CP and CP electrodes at the current densities of 1C.
Reproduced with permission.Copyright 2019, Elsevier. c) CV curves and EIS spectra of MoO2/MoS2@CC and pure carbon cloth. Reproduced with permission.Copyright 2020, Elsevier. d) Potentiostatic dischargei–tproﬁles at 2.09 V on different samples, and potentiostatic chargei–tproﬁles at 2.40 V on different samples for evaluation of Li2S dissolution behavior. Reproduced with permission.Copyright 2021, Elsevier.